 Nano Express
 Open Access
 Published:
PolarizationDependent QuasiFarField Superfocusing Strategy of NanoringBased Plasmonic Lenses
Nanoscale Research Letters volume 12, Article number: 386 (2017)
Abstract
The twodimensional superfocusing of nanoringbased plasmonic lenses (NRPLs) beyond the diffraction limit in the farfield region remains a great challenge at optical wavelengths. In this paper, in addition to the modulation of structural parameters, we investigated the polarizationdependent focusing performance of a NRPL employing the finitedifference timedomain (FDTD) method. By utilizing the state of polarization (SOP) of incident light, we successfully realize the elliptical, donut, and circularshape foci. The minimum full widths at half maximum (FWHMs) of these foci are ~0.32, ~0.34, and ~0.42 λ _{0} in the total electric field, respectively, and the depth of focus (DOF) lies in 1.41~1.77 λ _{0}. These subdiffractionlimit foci are well controlled in the quasifarfield region. The underlying physical mechanism on the focal shift and an effective way to control the focusing position are proposed. Furthermore, in the case of a high numerical aperture, the longitudinal component, which occupies over 80% of the electricfield energy, decides the focusing patterns of the foci. The achieved subdiffractionlimit focusing can be widely used for many engineering applications, including the superresolution imaging, particle acceleration, quantum optical information processing, and optical data storage.
Background
Along with the development of superresolution imaging [1], particle acceleration [2], quantum optical information processing [3], and polarizationdependent optical data storage [4], surface plasmonic devices are widely applied in these regions by modulating the plasmon resonance in a subwavelength magnitude. The plasmonic lens (PL), as a typical device, possesses the perfect imaging capability which was firstly proposed by J. B. Pendry in 2000 [5], and the subdiffractionlimit optical imaging was experimentally demonstrated by X. Zhang et al. 5 years later [6]. However, the imaging plane was confined to the extremely near field as the evanescent waves decrease exponentially, indicating a divergent optical field. This limitation makes it impracticable for standard optical microscopes [7].
In recent years, several nanostructurebased PLs have been investigated [8,9,10,11,12,13,14,15,16,17,18,19,20,21,22,23,24]. These PLs can not only realize the plasmonic focusing in plane [8] or in the near field [9] but can also possess the focusing ability in the far field [10,11,12,13] which were generally imaged by the scanning optical microscope [14]. However, these PLs showed a great difficulty to realize the focusing beyond the diffraction limit, until the dispersion relation of the metalinsulatormetal (MIM) waveguide was employed for the nanoslitbased PLs to modulate the phase at the subwavelength scale [11, 15,16,17]. The precise phase modulation contributes to the subdiffractionlimit focal line, and the linearly polarized light is generally applied as the incident light for these lenses. But, by simply extending the similar design method of onedimensional nanoslit lenses into two dimensions, the circularshape focus cannot be realized when the rotationally symmetric PL was illuminated by the linearly polarized light [18, 19], indicating the strongly polarization dependence of the focusing performance. Furthermore, the focal length was seriously deviated from the numerical calculation according to the wavefront reconstruction theory, especially for the nanoringbased PLs [18].
The nanoringbased PLs with the rotational symmetry, which are named as nanoringbased plasmonic lenses (NRPLs) for simplicity in the following discussion, are recognized as the substitution for the conversional refractive lenses in the subwavelength focusing systems. But from the perspective of the excitation of surface plasmon polaritons (SPPs), the linearly polarized light is unsuitable for the NRPLs as the excitation efficiency is proportional to the radial electricfield component of the incident light. Comparatively, the radially polarized light with the cylindrical symmetry in polarization adapts to the structural property of NRPLs [25]. Additionally, utilizing a donutshape aperture stop [26, 27] or Fresnel zone plate [28], this polarized light has been applied to realize the subwavelength circularshape focus. Thus, the radially polarized light was generally applied as the incident light of NRPLs [20,21,22,23]. Compared with the subwavelength focusing with the spatial filter, these PLs possess the ability to modulate the phase of incident light in the subwavelength waveguide. The excitation of surface plasmonic (SP) waves can enhance the transmission of electromagnetic waves. However, the superfocusing capability of plasmonic lens in the far field has not been demonstrated. Furthermore, although the composite NRPL has been proposed to modulate the focal length [24], the focal length failed to be effectively controlled and the electricfield energy is still concentrated in the center of the end surface of the lens.
In this paper, we present the theoretical design and numerical study of a NRPL, with the emphasis on the realization of superfocusing by utilizing the polarization property of incident light. We describe the theoretical design of NRPLs in our research and provide the focusing performance in the output region based on the finitedifference timedomain (FDTD) numerical simulation. To investigate the polarization dependence of the focusing performance, the linearly, circularly, azimuthally and radially polarized lights are all considered for illumination. We discuss the electricfield distribution features in the output region, including the subdiffractionlimit focusing, the shapes of foci, and the modulation of focal length, and point out the importance of the coaxial condition on the superfocusing performance.
Methods
The NRPLs investigated in this work were designed by using the wavefront reconstruction theory which was widely applied to the nanoslitbased PLs [11, 15]. In order to achieve the focus at the desired position, the relative phase delay caused when the light passes through the ith individual nanoring needs to satisfy the following condition based on the geometric optics:
where −Δϕ(r _{ i }) is the relative phase difference between the first nanoring in the inner center and the ith nanoring, r is the radius, λ _{0} is the freespace wavelength of the incident light, n is an arbitrary integer, and f _{0} is the designed focal length.
The basic comprising element of the surveyed NRPLs is the nanorings patterned in the metallic film. According to Ref. [29], when the diameter is larger than the wavelength of incident light, the air nanoring surrounded by metallic walls can be approximated to the MIM waveguide model as the inset illustrates in Fig. 1. The phase delay is primarily defined by the real part of the propagation constant β, expressed as Re(β)•t, where t is the thickness of the nanoring. Based on the dispersion relationship, the complex propagation constant β can be calculated as:
where k _{0} represents the wave vector in vacuum and ε _{ d } and ε _{ m } are the permittivity of dielectric and metal, respectively. Base on Eq. (2), we can see that the propagation constant β is dependent on the width of a nanoring. Thus, for the flat lens with a given thickness t, the caused phase delay is simply determined by the width w of the individual nanoring when the light passes through it. In our research, the dielectric is set to be air with the permittivity ε _{ d } = 1, and the gold film with a thickness t of 400 nm is employed, whose permittivity at the incident wavelength of 650 nm is ε _{ m } = −12.8915 + 1.2044i [15]. Additionally, as we previously reported [16], the coupling effect of the propagating lights in the two adjacent MIM waveguides also plays an important role on the phase delay, especially when the spacing metallic wall is smaller than twice the skin depth δ _{ m }, which can be estimated by [30]:
Accordingly, the calculated skin depth δ _{ m } is about 28 nm. By considering the coupling effect, a nanoslitbased PL with the superfocusing capability of 0.38 λ _{0} in resolution was reported in our previous research [16]. Here, to prominently analyze the influence of the state of polarization (SOP) on the focusing performance, the spacing walls between two adjacent nanorings are designed to be 100 nm, much larger than 2δ _{ m } to eliminate the coupling effect.
The schematic of the designed NRPL is shown in Fig. 2, and a total number of 32 concentric nanorings are included to reconstruct the wavefront. The width of the nanoring for the desired phase modulation range from 10 to 100 nm. The aimed focal length f _{0} is 1300 nm (2 λ _{0}). To efficiently utilize the MIM waveguide model, the minimum diameter of the innermost nanoring is set to be 800 nm. Furthermore, to avoid the focal shift as discussed in our previous work [15], the total phase difference is as large as 10π, with a predicted numerical aperture (NA) of 0.96. As a result, the theoretical Rayleigh diffraction limit, calculated by 0.61 λ _{0}/NA [31], is 413 nm (~0.64 λ _{0}).
To investigate the SOP influences of the incident light on the spatial intensity distributions, especially the focusing performance, the designed NRPL was illuminated by the linearly, circularly, azimuthally, and radially polarized light, respectively. All the cases were computed by the FDTD numerical simulations. According to the matrix optics, the different polarized lights can be described by the Jones matrix formalisms, and the corresponding matrix expression was applied to define the incident light. The boundary of the model was perfectly matched layer (PML) with a layer number of 12. To balance the computational accuracy and the memory consumption in the simulations, the mesh size was set to be 10 nm in the output region and 5 nm around the focal region.
Results
I Linear Polarization
For the linearly polarized light, the SOP is spatially homogeneous, and in this case, the direction of the electric vector is parallel to the x axis. When the light illuminates the NRPL, there exist two foci, distributing 400 nm away from each other in the total electric field E^{2} as presented in Fig. 3. Though the full widths at half maximum (FWHMs) of both are 210 nm (~0.32 λ _{0}) in the focal plane, the simulation result indicates that the intensity distribution is apparently different from the design based on the wavefront reconstruction theory where there should be a circulartype focus exactly on the z axis (also called the optical axis).
To analyze the differences between the simulation and theoretical design, the intensity distributions of the electricfield components are investigated. As presented in Fig. 4, there appears an ellipticalshape focus and the FWHM in x and ydirection is 220 nm (~0.34 λ _{0}) and 457 nm (~0.70 λ _{0}), respectively. This pattern agrees well with the experimental results of Ref. [18] where the same polarized light was applied. However, the simulation shows that the distribution pattern of E^{2} is similar to the pattern of the longitudinal component E _{ z }^{2} which occupies 79.8% of the total electric energy. Therefore, the difference is mainly attributed to the extraordinary distribution of E _{ z }^{2}.
This phenomenon can be ultimately explained by the transmission property of the NRPL. On the one hand, the excitation of SPPs at the interfaces of metal and dielectric generally depends on the local polarization direction of the incident light. The transverse electric (TE) waves cannot contribute to the excitation. On the other hand, due to the subwavelength structure of the MIM waveguide, only the SP waves can propagate through this lens [32]. With the rotational symmetry of the lens, the local transverse magnetic (TM) component changes with the azimuthal angle θ in the cosinoidal form. Therefore, as shown in Fig. 5a, the intensity distribution of E^{2}, which is just above the end surface of the lens, is concentrated in the near y = 0 region (−π/4 < θ < π/4). Correspondingly, the Poynting vectors propagate along the radial direction on the end surface, as presented in Fig. 5b. Thus, the vector direction of E is basically parallel to the optical axis, which forms the main content of E _{ z }. Due to the symmetrically constructive interference, there appear two foci in the focal plane instead of a circulartype focus.
II Circular Polarization
As the state of circularly polarized light changes with the time periodically, the simulated results are the timeaveraged field distribution. When the lens is illuminated by this polarized light, there forms a donutshape focus in E _{ z }^{2}. As shown in Fig. 6a, the focal length in this field is 1185 nm, showing a 8.85% deviation to the designed value. The width of the donut is 210 nm (~0.32 λ _{0}), and the radius is 400 nm. The depth of focus (DOF) is ~1.65 λ _{0}. The weight of E _{ z }^{2} is 80.6% of the total electric energy. Additionally, in E _{ r }^{2}, the superposition in the spatial domain generates a circular focus with the 1405nm focal length (a deviation of 8.08%). The FWHM is 295 nm (~0.45 λ _{0}) in this field, and the DOF is ~1.68 λ _{0}. Further, both distribution patterns in rz plane resemble those in the xz plane in the case of linearly polarized incident light. By taking into account the radial electricfield component, the FWHM can be reduced to 222 nm (~0.34 λ _{0}).
III Azimuthal Polarization
For the azimuthally polarized incident light, the electric vectors are perpendicular to the radial direction, which are parallel to the gold/vacuum interface of the NRPL. As the azimuthally polarized light illuminates the lens, the local TE waves fail to excite the SPPs on the interface. Thus, the transmission distance in nanorings is proportional to their widths as presented in Fig. 7. Since both the structure and illumination are of rotational symmetry, only half of the intensity distribution pattern and the structure of the NRPL are shown. The transmitted light can be neglected, and there is no distinct focus in the output region.
IV Radial Polarization
Corresponding to the azimuthally polarized light, the radially polarized light can be considered as the local TM wave, and this polarization property matches to the excitation condition of SPPs, which contributes to a higher maximum intensity at the focus. In total electric field E, the maximum intensity is five times larger than that for the linearly polarized incident light. Additionally, there is a circularshape focus with the 276nm (~0.42 λ _{0}) FWHM in E^{2}, as shown in Fig. 8. The simulated intensity distribution is much similar to the focusing capability of the high NA refractive lens [33]. Furthermore, this focusing performance is still dependent on E _{ z }^{2}, which occupies 82.0% of the total electric energy.
Different from the former cases, there is a circularshape focus in E _{ z }^{2}. Besides, this component also determines the distribution pattern in E^{2}. As presented in Fig. 9a, the FWHM in E _{ z }^{2} is 260 nm (~0.40 λ _{0}) which is close to that of the focal line in the case of nanoslitbased PL [16]. Particularly, the focal length is 1275 nm. Compared with the designed value, the relative error decreases to 1.9%. However, the focal length is 1455 nm (a deviation of 11.2%) in E _{ r }^{2}. As presented in Fig. 9b, there is a donutshape focus with the 227nm width (~0.35 λ _{0}) in this field. The DOF is ~1.60 λ _{0}.
The phase delay of the SP waves in nanorings is investigated, as presented in Fig. 10. The simulation indicates that the phase modulation is dramatically influenced by the structural parameters of the NRPL and the simulated phase delays between the incident surface and the output surface are basically identical to the calculated values based on Eq. (2). On the end surface of the lens, the SP waves still propagate along the radial direction and there is a hot spot at the center of the surface, whose intensity is one fifth of the focus intensity. The constructive interference of the SP waves, with the rotational symmetric distribution, constructs the propagating waves and realizes the circularshape focus in the quasifar field.
Discussions
I Superfocusing Capability of NRPLs
As the incident lights with different SOPs are applied, including the linear, circular, and radial polarizations, the subdiffractionlimit foci can be realized. Although the focus shape is influenced by the SOP, the characteristic sizes of these foci all overcome the Rayleigh diffraction limit (413 nm). The simulation results successfully demonstrate the superfocusing capability of the NRPL, and the intensity distribution in the focal plane is similar to the Bessel function which is used to describe the nondiffraction beam.
For the case of the radially polarized incident light, as an example shown in Fig. 11, the intensity distribution in E _{ z }^{2} is identical to the zeroorder Bessel function J _{0}(K _{ spp } ⋅ n ⋅ r), where n and r is the refractive index of the environmental medium and the radial distance to the optical axis, respectively. The FWHM of the focus is slightly larger than the size of the main lobe calculated with J _{0}. Particularly, the simulations indicate that the nondiffraction beam can be realized in the quasifar field. The SP waves, as a kind of evanescent wave, are decreased exponentially when propagating away from the exit surface, and the propagating distance in the vacuum can be calculated by [30]:
where ε _{d} and ε _{m} are the permittivity of dielectric and metal, respectively. Thus, δ _{d} is 357 nm which is consistent with the simulation as shown in Fig. 8d. Therefore, the intensity of the SP waves at the focus can be neglected in the quasifarfield region.
II Shape of Focus
By modulating the SOP, the elliptical, circular, and donutshape foci can be realized in the focal plane, as presented in Fig. 12. The phenomenon is attributed to the subwavelength focal size, and we cannot realize the circulartype focus in both electric and magnetic fields at the same time. Thus, a donuttype focus is realized in the magnetic (or electric) fields, while a circulartype focus is achieved in the correspondingly electric (or magnetic) field. Particularly, because there is no longitudinal magnetic field, the intensity distribution of H^{2} is the same as the pattern of E _{ r }^{2}. Furthermore, E _{ z }^{2} occupies about 80.0% of the total electric energy and the scale is not affected by the SOPs of the incident light.
III Modulation of Focal Length
The simulated focal length in different cases is basically close to the desired position f _{0} (1300 nm), as shown in Table 1. But, we realize that the focal length in the transverse field E _{ r }^{2} is about 200 nm longer than that in the longitudinal field E _{ z }^{2}, regardless of the SOP of the incident light and the deviation commonly exists.
In theory, the wavefront reconstruction theory is suitable for designing the NRPL with an arbitrary focal length from the nearfield to the farfield region. However, whether the actual focal length of a designed plasmonic lens agrees well with the designed focal length depends on the total phase difference of the lens. The deviation may attribute to the distinction between the amplitudetype focus and phasetype focus [34]. Because the phase modulation in the MIM waveguide aims for the radial component, the focal length in E _{ r }^{2} can be modulated by the wavefront reconstruction theory, when the total phase difference of at least 2π is satisfied [15]. For the longitudinal component, a larger total phase difference (>10π) is advantageous to the consistency. As shown in Fig. 13, when the phase difference increases from 2π to 16π, correspondingly the NA of 0.75 to 0.96, the amplitudetype focus in E _{ z }^{2} moves from the output surface of the lens to the desired position. As the intensity distribution of E^{2} is decided by E _{ z }^{2}, the NA can dramatically influence the focal length in the total electric field. However, the change of the focal length in E _{z}^{2} decreases gradually, along with the increase of the total phase difference. On the other hand, the position of the phasetype focus in E _{ r }^{2} is relatively stable. When the NRPL with a high NA is applied, there is still a deviation in focal length derived based on the intensity distribution of E _{ x }^{2} and E _{ z }^{2}, and the deviation almost keeps invariable. Therefore, the focal length of the NRPLs can be effectively controlled by the phase modulation and structural optimization, though the same focal length cannot be achieved in the transverse and longitudinal component fields.
IV Focusing Performace in the NonCoaxial Situation
The noncoaxial situation is a common problem in the experiment, and its effect on the focusing performance should be considered. As shown in Fig. 14, the center of the radially polarized light deviates 3 μm from the optical axis of the NRPL along the x axis. Compared with Figs. 8 and 9, the intensity distributions both in xz cross section and in focal plane are apparently changed. In the longitudinal electric field, an elliptical focus is located at 1340 nm away from the exit surface of the lens. The FWHMs in xz and yz planes are 0.51 and 0.38 λ _{0}, respectively. On the other hand, the distribution in transverse field is also distorted, where the intensity of one side lobe is higher than the other one. Furthermore, compared with the coaxial condition, the decrease of the maximum intensity in the total electric field is more than 85%.
The preliminary simulation indicates that the noncoaxial situation indeed influences the intensity distribution and the desired focusing performance of lens. Therefore, it is essential to guarantee the coaxiality between the incident light and the lens center during the experiment.
Conclusions
In summary, we build a NRPL with a high NA utilizing the wavefront reconstruction theory and the dispersion relation of the MIM waveguide. We also investigate the polarizationdependent focusing performance in the quasifar field, including the focal length, FWHM, DOF, and the maximum intensity. The conventional polarized light, such as the linearly, circularly, radially, and azimuthally polarized light, are all considered. The simulations demonstrate the superfocusing capability of the designed NRPL. Utilizing the polarizationdependent property, the subdiffractionlimit elliptical, circular, and donutshape foci can be realized. However, one limitation of this work is that the proposed design strategy to realize the superfocusing performance of NRPLs is aimed for the quasifarfield region, although to the best of our knowledge, the similar focusing capability in this region is rarely reported. In addition, we discover the underlying physical phenomenon on the focal shift and propose a more effective way to control the focusing position by employing both the transverse and longitudinal fields. There are considerable engineering applications for the nanoringbased superfocusing lenses, ranging from the superresolution imaging, particle acceleration, quantum optical information processing to the optical data storage.
Abbreviations
 DOF:

Depth of focus
 FDTD:

Finitedifference timedomain
 FWHM:

Fullwidth at half maximum
 MIM:

Metalinsulatormetal
 NRPL:

Nanoringbased plasmonic lenses
 PML:

Perfectly matched layer
 SOP:

State of polarization
 SPPs:

Surface plasmon polaritons
 TE:

Transverse electric
 TM:

Transverse magnetic
References
Gjonaj B, Aulbach J, Johnson PM, Mosk AP, Kuipers L, Lagendijk A (2013) Focusing and scanning microscopy with propagating surface plasmons. Phy Rev Lett 110(26):919–919
Kar S, Ahmed H, Prasad R, Cerchez M, Brauckmann S, Aurand B, Cantono G, Hadjisolomou P, Lewis CLS, Macchi A, Nersisyan G, Robinson APL, Schroer AM, Swantusch M, Zepf M, Willi O, Borghesi M (2016) Guided postacceleration of laserdriven ions by a miniature modular structure. Nat Commun 7:10792
Rui GH, Zhan QW (2016) Tailoring optical complex fields with nanometallic surfaces. Nanophoton 4(1):2–25
Cui Y, Phang IY, Hegde RS, Lee YH, Ling XY (2014) Plasmonic silver nanowire structures for twodimensional multipledigit molecular data storage application. ACS Photon 1(7):631–637
Pendry JB (2000) Negative refraction makes a perfect lens. Phys Rev Lett 85(18):3966–3969
Fang N, Lee H, Sun C, Zhang X (2005) Subdiffractionlimited optical imaging with a silver superlens. Science 308(5721):534–537
Simkhovich B, Bartal G (2014) Plasmonenhanced fourwavemixing for superresolution applications. Phys Rev Lett 112(5):755–759
Fang ZY, Lin CF, Ma RM, Huang S, Zhu X (2010) Planar plasmonic focusing and optical transport using CdS nanoribbon. ACS Nano 4(75):75–82
Bao YJ, Zu S, Liu W, Zhou L, Zhu X, Fang ZY (2017) Revealing the spin optics in conicshaped metasurfaces. Phys Rev B 95:081406(R)
Lin L, Goh XM, McGuinness LP, Roberts A (2010) Plasmonic lenses formed by twodimensional nanometric crossshaped aperture arrays for Fresnelregion focusing. Nano Lett 10(5):1936–1940
Verslegers L, Catrysse PB, Yu Z, White JS, Barnard ES, Brongersma ML, Fan S (2009) Planar lenses based on nanoscale slit arrays in a metallic film. Nano Lett 9(1):235–238
Ishii S, Shalaev VM, Kildishev AV (2013) Holeymetal lenses: sieving single modes with proper phases. Nano Lett 13(1):159–163
Yu YT, Wang P, Zhu YC, Diao JS (2016) Broadband metallic planar microlenses in an array: the focusing coupling effect. Nanoscale Res Lett 11(1):109
Gjonaj B, David A, Blau Y, Spektor G, Orenstein M, Dolev S, Bartal G (2014) Sub100 nm focusing of short wavelength plasmons in homogeneous 2D space. Nano Lett 14(10):5598–5602
Yu YT, Zappe H (2011) Effect of lens size on the focusing performance of plasmonic lenses and suggestions for the design. Opt Express 19(10):9434–9444
Zhu YC, Yuan WZ, Yu YT, Diao JS (2015) Metallic planar lens formed by coupled widthvariable nanoslits for superfocusing. Opt Express 23(15):20124–20131
Zhu YC, Yuan WZ, Yu YT, Wang P (2016) Robustly efficient superfocusing of immersion plasmonic lenses based on coupled nanoslits. Plasmonics 11(6):1–6
Liu Y, Xu H, Stief F, Zhitenev N, Yu M (2011) Farfield superfocusing with an optical fiber based surface plasmonic lens made of nanoscale concentric annular slits. Opt Express 19(21):20233–20243
Diao JS, Yuan WZ, Yu YT, Zhu YC, Wu Y (2016) Controllable design of superoscillatory planar lenses for subdiffractionlimit optical needles. Opt Express 24(3):1924–1933
Wang H, Shi L, Lukyanchuk B, Sheppard C, Chong CT (2008) Creation of a needle of longitudinally polarized light in vacuum using binary optics. Nat Photon 2(8):501–505
Lerman GM, Yanai A, Levy U (2009) Demonstration of nanofocusing by the use of plasmonic lens illuminated with radially polarized light. Nano Lett 9(5):2139–2143
Chen W, Abeysinghe DC, Nelson RL, Zhan QW (2009) Plasmonic lens made of multiple concentric metallic rings under radially polarized illumination. Nano Lett 9(12):4320–4325
Qi J, Kaiser T, Klein AE, Steinert M, Pertsch T, Lederer F, Rockstuhl C (2015) Enhancing resonances of optical nanoantennas by circular gratings. Opt Express 23(11):14583–14895
Yu P, Chen SQ, Li JX, Cheng H, Li ZC, Liu WW, Tian JG (2015) Dynamically tunable plasmonic lens between the near and far fields based on composite nanorings illuminated with radially polarized light. Plasmonics 10(3):625–631
Zhan QW (2009) Cylindrical vector beams: from mathematical concepts to applications. Adv Opt Photon 1(1):1–57
Kitamura K, Sakai K, Noda S (2010) Subwavelength focal spot with long depth of focus generated by radially polarized, narrowwidth annular beam. Opt Express 18(5):4518–4525
Stadler J, Stanciu C, Stupperich C, Meixner AJ (2008) Tighter focusing with a parabolic mirror. Opt Lett 33(7):681–683
Liu T, Liu Q, Yang SM, Jiang ZD, Wang T, Yang XK (2017) Shaping a farfield optical needle by a regular nanostructured metasurface. Opt Commun 393:72–76
Cai L, Zhang J, Bai W, Wang Q, Wei X, Song G (2010) Generation of compact radially polarized beam at 850 nm in verticalcavity surfaceemitting laser via plasmonic modulation. Appl Phys Lett 97(20):201101
Raether H (1988) Surface Plasmons on Smooth and Rough Surfaces and on Gratings (SpringerVerlag
Huang K, Ye H, Teng J, Yeo SP, Luk’yanchuk B, Qiu CW (2013) Optimizationfree superoscillatory lens using phase and amplitude masks. Laser & Photon Rev 8(1):152–157
Dan’ko V, Dmitruk M, Indutnyi I, Mamykin S, Myn’ko V, Shepeliavyi P, Lukaniuk M, Lytvyn P (2017) Au gratings fabricated by interference lithography for experimental study of localized and propagating surface plasmons. Nanoscale Res Lett 12(1):190
Youngworth KS, Brown TG (2000) Focusing of high numerical aperture cylindricalvector beams. Opt Express 7(2):77–87
Saeidi C, Weide DVD (2015) A figure of merit for focusing metasurfaces. Appl Phys Lett 106(11):4542–4552
Acknowledgements
The authors acknowledge the financial support by the National Natural Science Foundation of China (Grant No. 51375400, 51622509); the Specific Project for the National Excellent Doctorial Dissertations (Grant No. 201430); the 111 Project (Grant No. B13044); Innovation Foundation for Doctor Dissertation of Northwestern Polytechnical University (CX201606); and the Seed Foundation of Innovation and Creation for Graduate Students in Northwestern Polytechnical University (Z2017013).
Authors’ Contributions
The idea of the study was conceived by HS, YZ, and YY. SH carried out the total numerical simulation of the superfocusing performance and the polarizationdependent properties of NRPLs and finished the first draft. The structure of the simulated model was modulated with the help of BG and PW. This manuscript was finally finished after the adjustment about this article logical proposed by YY. All the authors read and approved the final manuscript.
Competing Interests
The authors declare that they have no competing interests.
Publisher’s Note
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Author information
Authors and Affiliations
Corresponding author
Rights and permissions
Open Access This article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.
About this article
Cite this article
Sun, H., Zhu, Y., Gao, B. et al. PolarizationDependent QuasiFarField Superfocusing Strategy of NanoringBased Plasmonic Lenses. Nanoscale Res Lett 12, 386 (2017). https://doi.org/10.1186/s1167101721541
Received:
Accepted:
Published:
DOI: https://doi.org/10.1186/s1167101721541
Keywords
 Polarization
 Nanoringbased plasmonic lenses
 Subwavelength structures
 Superfocusing
 Geometric optics